Journal of Dental Biomaterials. 2017;4(2) Original Article
Evaluation of Compressive Strength and Sorption/Solubility of Four Luting Cements Tavangar MSa, Jafarpur Db, Bagheri Rc* Department of Dental Materials, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran Student Research Committee, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran c Department of Dental Materials and Biomaterials Research Center, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran a
Article History: Received: 8 April 2017 Accepted: 30 May 2017
Statement of Problem: Compressive strength (CS) and sorption/solubility of the luting cements are two associated factors. Searching a correlation between sorption/solubility and compressive strength of various luting cements is required. Objectives: To measure the water sorption/solubility, and compressive strength of three resin-based and one conventional glass ionomer (CGI) luting cement after 1 and 24 h of immersion in distilled water and to determine if there is any correlation between those properties found. Materials and Methods: Four luting cements were investigated. For each material, 10 disc shaped specimens were prepared for measuring the sorption/ solubility. The specimens were cured according to the manufacturer’s instructions, and the sorption/solubility were measured in accordance with the ISO 4049’s. For testing the compression strength, for each material 16 cylindrical specimens were prepared by insertion of cements into a stainless steel split mould. The specimens were cured, divided into groups of 8, and then stored in distilled water at (37 ± 1)°C for 1 and 24 h. The test was performed using the universal testing machine, the maximum load was recorded and CS was calculated. The data were analysed using SPSS software version 18. Oneway ANOVA, post-hoc Tukey’s test and Pearson’s correlation coefficient were performed. Results: G-CEM had the highest mean CS (153.60± 25.15) and CGI luting had the lowest CS (21.36±5.37) (p 0.05). The lowest mean sorption/solubility value was for RelyXTM U200 and Panavia F, and the highest for CGI luting (all p < 0.001). Conclusions: The compressive strength of all cements did not necessarily increase after 24 h and varied depending on the materials. There was a strong reverse correlation between sorption and CS values after both 1 and 24 h immersion. It may be practical for clinician to use those cements with the less sorption / solubility and more stable compression strength over time.
Key words: Compression Strength Resin Luting Cements Sorption/Solubility Corresponding Author: Rafat Bagheri Department of Dental Materials and Biomaterial Research center, Shiraz University of Medical Sciences, Shiraz, Iran Email: [email protected]
, [email protected]
Tel: +98-71-36280119 Fax: +98-71-36285276
Cite this article as: Tavangar M, Jafarpur D, Bagheri R. Evaluation of Compressive Strength and Sorption/Solubility of Four Luting Cements. J Dent Biomater, 2017;4(2):387-393.
Mechanical Properties of Luting Cements
Introduction Several categories of the luting cements are being used for cementation of direct or indirect restorations to the tooth structure . Water based cements such as zinc phosphate and polycarboxylate cements have been used for a long time as the main luting agent for the cementation of restoration. Since 1972  when it was introduced, glass ionomer cements have gained popularity due to their clinical advantages including fluoride release and their adhesion capabilities to the tooth structure . However, poor early mechanical properties and moisture sensitivity are considered as disadvantages of these materials . The resin luting cements are the latest type of luting agents for the cementation of indirect aesthetic restorations such as all-ceramic and porcelain veneers. Resin cements are classified into two types: conventional and self-adhesive resin luting cements. The self-adhesive resin luting cements (SARLC) have the ability to bond to the tooth structure and the internal surface of the restoration without using adhesive system. Resin luting cements are comprised of the same basic constituents as the composite restorative material but with lower concentration of filler particles with a variable amount of 55–70 W% . Resin cements have advantages of colour stability, adhesion to dental structure and other materials, low water sorption and solubility, and better mechanical properties in comparison to traditional cements [6-8]. There are also major disadvantages, such as polymerization shrinkage . Luting cements seal the interface of the indirect restoration and the prepared tooth surface; hence, the clinical success of the restoration depends on the mechanical and physical properties of the luting cements over the duration of the restoration . These materials are subjected to forces of mastication and transferring the stresses from indirect restorations to the tooth structure. Therefore, it is necessary for luting cement to provide high strength in order to maintain the durability and success of the restorations [10,11]. In addition to the mechanical properties, other clinically related characteristics including dimensional stability and structural integrity should be considered for the selection of a durable luting agent . To maintain the dimensional stability, luting cement should have adequate resistance to fracture and deterioration when exposed to the oral cavity fluids . Water sorption and solubility may cause
degradation of the cement, leading to disintegration in margin of the restorations. Clinically, loss of marginal integrity can cause unwanted consequences such as marginal leakage and discoloration, secondary caries, hypersensitivity, releasing toxic substances, and finally may result in debonding or the fracture of the restoration [3,12]. Previous studies reported comparable moisture sensitivity for the resin modified (RMGIC) with conventional glass ionomer cements . Knobloch et al.  investigated sorption and solubility of 3 RMGICs and 3 resin cements reported that water sorption was significantly higher in all RMGICs as compared to resin cements, attributing it to the hydrophilic nature of HEMA in the composition of RMGICs . Similarly, by evaluating the sorption and solubility of eight luting agents (two RMGICs and six resin cements) in distilled water and ethanol, Mese et al. found that RMGICs exhibited higher solubility and sorption as compared to resin cements . Although the resin luting cement showed lower water sensitivity, the weakening of their mechanical properties has been reported after water storage . Water is mainly absorbed by the polymer matrix, leading to hydrolytic degradation, debonding of the fillers, and matrix softening. When the resin matrix starts swelling because of water sorption, unreacted monomers and deboned fillers may leach out from the matrix. Consequently, moist conditions can decrease the final strength and increase the creep . Örtengren et al.  studied the effect of 60 days of water sorption on the flexural strengths of two resin cements. Their findings showed that after water storage, resin cement revealed significantly lower flexural strength and higher deflection which may be explained by the plasticizing effect of water on the polymers. Several studies have compared the mechanical properties, and water sorption / solubility of different classes of luting cements [11,12]. Yet, the correlation between water sorption and solubility of various categories of luting cements and their compressive strength has not been widely studied. Therefore, the present study aimed to place various luting cements in distilled water and determine: 1) the effect of 1 and 24 h immersion on the compressive strength; 2) water sorption/solubility of those cements in accordance with the ISO 4049’s; 3) if a correlation exists between the sorption/solubility and the compressive strength of the luting cements. jdb.sums.ac.ir J Dent Biomater 2017;4(2)
Tavangar MS et al.
The null hypothesis is that the storage time does not affect compressive strength, or there is no correlation between the compressive strength and water sorption/ solubility of the cements. Materials and Methods Four luting cements were investigated in this study, as shown in Table 1.
right angles to each other were made and the area (in square millimetres) was calculated by using the mean diameter. By measuring the thickness of the specimen at the centre of the specimen and at four equally spaced points on the circumference, the volume, V, was calculated in cubic millimetres as follows: V= π × (d/2)2 × h, where π =3.14, d is the mean diameter and h is the mean thickness of the specimen. The specimens of each material were immersed in distilled
Table 1: Description of the materials Cement
RelyXTM U200 Automix syringe
3MESPE,St. Paul, MN, USA
Panavia F 2 pastes
Kuraray Noritake Dental Inc., Okayama, Japan
GC corporation, Tokyo Japan
CGI luting & lining cement Powder and liquid
GC corporation, Tokyo Japan
SARLC= Self Adhesive Resin Luting Cement, SGIC= Conventional Glass Ionomer luting Cement, CRLC= Conventional Resin Luting Cement.
Water sorption and Solubility test For each material, 10 disc-shaped specimens of 10 ± 0.1mm of diameter and 1.0 ± 0.1mm of thickness were prepared. A polyethelyn mould was filled with the material according to the manufacturer’s instructions. Then, the mould was sandwiched between two pieces of Mylar strip and pressed by two glass plates under hand pressure to remove the excess material. The light cured specimen were eradicated for the recommended exposure time trough Mylar strip using LED curing unit at a wavelength range of 440-480nm and an emitting light intensity of 1500 mW/cm2 (Radii plus LED; SDI, Melbourne, Victoria, Australia). In accordance with the ISO 4049’s instructions , the specimens were transferred to a desiccator (Labx Company, Ontario, Canada) containing freshly dried silica gel (SIGMA-ALDRICH, Taufkirchen, Germany) maintained at (37± 1)°C. After 22 h, the specimens were removed and transferred to a second desiccator maintained at (23±1)°C for another 2 h. After 24 h, the specimens were removed and weighed on an electronic balance (GR-3000, A & D CL Toshiba, Tokyo, Japan) to an accuracy of ± 0.1mg. This procedure was repeated every 24 h until a constant mass, m1, was obtained. After the final drying, two measurements of the diameter at the
jdb.sums.ac.ir J Dent Biomater 2017;4(2)
water at (37± 1)°C for 7 d. After this time period, the specimens were removed, washed with distilled water, air dried and then weighed in one minute and recorded as m2. The specimens were reconditioned to a constant mass in the desiccator. The constant mass was recorded as m3. The values for water sorption, Wsp , and solubility, Wsl, in µg/mm3, was calculated using the following equations:Wsl=(m1-m3)/V and Wsp =(m2-m3) / V where m1 is the conditioned mass prior to immersion in water; m2 is the mass of the specimenafter immersion in water for 7 d; m3 is the mass of the reconditioned specimen (all in micrograms); and V is the volume of the specimen, in cubic millimetres. Compression test For each material, 16 cylindrical specimens of 4.0 mm in diameter and 8.0 mm long were prepared by insertion of cements into a stainless steel split mould. The light cure materials were cured according to the manufacturer’s instruction by the same LEDcuring unit mentioned above. The specimens were removed from the split mould and cured with the same exposure time on the opposite side and each lateral face. The specimens were divided into groups of 8
Mechanical Properties of Luting Cements
Table 2: Mean ± SD (MPa) of compressive strength for all luting cements analysed using Tukey’s test Luting cement
138.50 ± 22.8 A
129.20 ± 19.92 A
110.07 ± 47.5 A
162.33 ± 22.00 A
153.60 ± 25.15 A
162.60 ± 18.48 A
21.36 ± 5.37 B
30.50 ± 22.78 B
- In each column, mean values with different upper case letters show a significant difference (p value< 0.05). *shows significance level of student’s t test between two storage time in each material.
(n=8) and then stored in distilled water at (37 ± 1)°C for one and 24 h. Following the storage, the compression strength test was performed using the universal testing machine (Zwick/Roll Z020, Zwick GmbH & Co, Germany) loaded at a crosshead speed of 0.5mm/min. The maximum load at specimen failure was recorded and compressive strength was calculated using the following formula: δ=F/S where F is the maximum load at the fracture point (N) and S is the surface area of the specimen (mm2). Data Analysis The data were analysed using SPSS software version 18 (SPSS Inc., Chicago, IL, USA). One-way ANOVA was used to compare different variables between the materials, and post-hoc Tukey’s test was performed to show significant differences in subgroup comparisons. Student’s t test was used to show significant differences between the two storage times for compressive strength of each material. Correlations between sorption/solubility and compressive strength were assessed using Pearson’s correlation coefficient. p value of < 0.05 was considered to be statistically Table 3: Mean ± SD (μg/mm3) of sorption and solubility for all luting cements analysed using Tukey’s test Luting cements
significant. Results As shown in Table 2, after 1 h of immersion in distilled water, the highest mean CS value was observed for G-CEM (153.6 ± 25.15), followed by RelyXTM U200 (138.5 ± 22.8) and Panavia F (110.07 ± 47.5). CGI luting showed the lowest mean CS (21.36 ± 5.37) (p < 0.001). After 24 h, mean CS values were numerically but not statistically raised for all the cements except for RelyXTM U200 which showed a slight reduction. After 24 h, CS values for Panavia F increased as high as G-CEM with the following order: G-CEM=Panavia F > RelyXTM U200 > CGI luting. Table 3 compares the water sorption and solubility of all tested cements. The lowest mean sorption value was for RelyXTM U200 (23.6 ± 1.59) and Panavia F (24.10 ± 6.87). The highest mean sorption value was for CGI luting (76.20 ± 6.17) (p < 0.001). The lowest mean solubility value was found to be for RelyXTM U200 and Panavia F followed by G-CEM, and CGI luting, respectively (p < 0.001). There was a strong reverse correlation between sorption and CS values after both 1 and 24 h of immersion (r = -0.702, p = 0.002; and r = -0.775, p < 0.001, respectively). Solubility showed a moderate reverse correlation with CS values after 1 h (r = -0.530, p = 0.035) and no significant correlation after 24 h (r = -0.409, p = 0.116).
23.61 ± 1.59A
1.23 ± 0.83A
24.10 ± 6.87A
8.40 ± 4.28AB
38.90 ± 4.59B
17.29 ± 9.55BC
76.20 ± 6.17C
27.97 ± 2.11C
Compressive strength and sorption/solubility are correlated factors which enhance the longevity of bonded restorations when they are in an optimum level. A high compressive strength of the luting cements enables them to withstand masticatory forces in the mouth and increases the fracture resistance of
- In each column, mean values with different upper case letters show a significant difference (p value< 0.05). (p < 0.05).
jdb.sums.ac.ir J Dent Biomater 2017;4(2)
Tavangar MS et al.
the restoration, especially in brittle materials such as ceramics . In this experiment, compressive strength and water sorption/solubility of two self- adhesive resin luting cements (SARLC), one conventional resin luting cement (CRLC), and one conventional glass ionomer (CGI) luting were examined and compared. In general, CGI luting exhibited significantly lower compressive strength and higher water sorption / solubility than both SARLC and CRLC. Comparison of the resin cements showed that CRLC had a lower strength than SARLC but it showed a comparable or less water sorption / solubility. As shown in Table 2, compressive strength of all materials showed an increase after 24 h of immersion in distilled water except for RelyXTM U200 which revealed a slight decrease after 24 h. The increase in the materials’ strength after 24 h can be related to their setting reaction. For glass ionomer cements, after mixing, the calcium polycarboxylate is formed in the first few minutes while the aluminum polycarboxylate, which improves the mechanical properties of the cement, takes at least 24 hours or even longer to be formed [16-18]. Likewise, for resin-based materials, polymerization and maturation take 24 h to be completed. Therefore, the mechanical properties of these materials are expected to be improved significantly after 24 hours. In the present study, one of the SARLC (RelyXTM U200) had a slight reduction from ≈138 to ≈129 MPa while the other one (G-CEM) had a slight increase from ≈153 to ≈162 MPa. The CRLC, Panavia F, showed the lowest compressive strength (≈110 MPa) among resin-based cements after 1 h of setting while after 24 h of setting, it had a remarkable increase (≈162 MPa) that was equal to the highest value for G-CEM. These results suggest that the growth in the luting cements’ strength is not directly dependent on the period of 24 h of setting. The effect of 24 h of immersion in distilled water on the compressive strength of the resin cements varied depending on the materials. Some materials showed a slight reduction and some others significant increase in strength after 24 h of immersion. This result is in agreement with that of a previous study . A previous study  evaluating the shear punch strength of resin cements reported a reduction of strength for almost all SARLCs after one week, one month and even more after three months of immersion in distilled water. While Panavia F with HEMA 391
jdb.sums.ac.ir J Dent Biomater 2017;4(2)
content in their composition showed an increase after one-week of immersion, it has been concluded that the HEMA could be a major factor in the reinforcement or stiffness of the polymer system . It has been shown  that the water sorption of a SARLC (Maxcem) was significantly higher than a CRLC (Panavia F). It has also been hypothesized that the significant decrease in the strength of SARLC might be related to its greater water sorption than CRLC . However, the results of our study did not prove this claim. The water sorption / solubility of the tested luting cements followed the following trend: RelyXTM U200 < Panavia F < G-CEM< CGI luting. This result reveals that although G-CEM had the greatest water sorption/ solubility among other resinbased cements, did not drop the strength but also exhibited the highest strength value either after 1 or 24 h of immersion in water. On the other hands, RelyXTM U200 with the least sorption and solubility exhibited the lowest strength after 24 h of immersion. In other words, G-CEM with higher strength than RelyXTM U200 had higher water sorption and solubility. Hence, it is speculated that having a high water sorption/solubility does not necessarily decrease the compressive strength of resin luting cements. But, some factors other than sorption/solubility, such as polimerization, mode of curing (dual- or self-cure), and degree of conversion (%DC) might have a great influence on the strength  or sorption/ solubility  of the resin luting cements. Factors that may affect polymerization include cement film thickness, opacity, and translucency of both the cement and restoration. Properly cured resin cement will exhibit high compressive and flexural strengths and less solubility in the oral fluids. The mixing method of the resin cement is also an important clinical factor that improves the performance of the resin cement . Although resin cements are insoluble in oral fluids, being resins, they absorb water. Due to water sorption, the flexural strength of the resin cements is decreased . The flexural strength affected by the thickness of the cement, the greater decrease occurred in the greater film thickness of the cement because it makes the cement unable to scatter stresses from masticatory function between the tooth and restoration. Therefore, keeping the resin cement layers to a thin layer minimizes the plasticizing effect in the resin cements . In the present study, Panavia F (a dual-cure luting cement) showed significantly less sorption/solubility than G-CEM (a light cure luting cement) which can
Mechanical Properties of Luting Cements
be due to their different mode of curing. A recent study  investigated the effect of curing mode on the surface energy and sorption/solubility of SARLC and CRLC and found a greater sorption/solubility values for SARLC than the CRLC. The author concluded that the degree of conversion (%DC) was negatively correlated with the sorption/solubility values. Dual curing is shown to reduce the sorption and/or solubility in comparison with self-curing by increasing %DC . The convention glass ionomer used in this study (CGI Lutin) exhibited the lowest strength and the highest sorption and solubility. It is well known that water has an important role in the glass ionomer cement. It contributes to the transportation of calcium and aluminum cations, reacting with the polyacid to form a polyacrylate matrix . During the early stage of maturation, moisture contamination leads to loss of components, decrease of physical properties and loss of translucency . After hardening, desiccation and loss of water results in the inadequacy of the reactions and surface crazing . Therefore, it is expected to absorb and lose water easily.
Conclusions Within the limitations of this study, the following conclusions were drawn. In general, most of the cements showed an increase in the compressive strength after 24 h immersion in comparison with the 1 h immersion except for RelyXTM U200 that had a slight decrease. RelyXTM U200 and Panavia F, revealed the lowest sorption / solubility and CGI luting the highest. There was a strong reverse correlation between sorption and CS values after both 1 and 24 h immersion. Based on the results of this study, it is speculated that it may be practical for clinician to use those cements with the less sorption / solubility and more stable compression strength over time.
13. Acknowledgments The authors would like to thank the Vice Chancellor for Research Affairs of Shiraz University of Medical Sciences for financial support of the research.
Conflict of Interest: None declared. 15. References 1. Giti R, Vojdani M, Abduo J, et al. The Comparison
of Sorption and Solubility Behavior of Four Different Resin Luting Cements in Different Storage Media. J Dent (Shiraz). 2016;17:91-97. Wilson AD, Kent BE. A new translucent cement for dentistry. The glass ionomer cement. Br Dent J. 1972;132:133-135. Knobloch LA, Kerby RE, McMillen K, et al. Solubility and sorption of resin-based luting cements. Oper Dent. 2000;25:434-440. Bagheri R, Taha NA, Azar MR, et al. Effect of G-Coat Plus on the mechanical properties of glass-ionomer cements. Aust Dent J. 2013;58:448-453. Simon JF, Darnell LA. Consideration for proper selection of dental cements. Compend Contin Educ Dent. 2012;33:28–36. Rueggeberg FA, Caughman WF. The influence of light exposure on polymerization of dual-cure resin cements. Oper Dent. 1993;18:48–55. Suzuki S, Minami H. Evaluation of toothbrush and generalized wear of luting materials. Am J Dent. 2005;18:311-317. Kumbuloglu O, Lassila LV, User A, et al. A study of the physical and chemical properties of four resin composite luting cements. Int J Prosthodont. 2004;17:357-363. Radovic I, Monticelli F, Goracci C, et al. Selfadhesive resin cements: a literature review. J Adhes Dent. 2008;10:251-258. Patil SG, Sajjan MS, Patil R. The effect of temperature on compressive and tensile strengths of commonly used luting cements: an in vitro study. J Int Oral Health. 2015;7:13-19. Li ZC, White SN. Mechanical properties of dental luting cements. J Prosthet Dent. 1999;81:597609. Mese A, Burrow MF, Tyas MJ. Sorption and solubility of luting cements in different solutions. Dent Mater J. 2008;27:702-709. Azar MR, Bagheri R, Burrow MF. Effect of storage media and time on the fracture toughness of resin-based luting cements. Aust Dent J. 2012;57:349-354. Ortengren U, Elgh U, Spasenoska V, et al. Water sorption and flexural properties of a composite resin cement. Int J Prosthodont. 2000;13:141147. ISO 4049:2000 (E). Dentistry-polymer-based filling, restorative and luting materials; 7.12 Water sorption and solubility. International Organization for Standardization; 2000. Available jdb.sums.ac.ir J Dent Biomater 2017;4(2)
Tavangar MS et al.
at: https://www.iso.org/standard/23041.html Powers JM, Farah JW, O’Keefe KL, et al. Guide to all-ceramic bonding. Available from: http:// www.Kuraraydental.com/guides/-item/guide-toall-ceramic-bonding: 2013. Oilo G. Early erosion of dental cements. Eur J Oral Sci. 1984;92:539-543. Pearson GJ, Atkinson AS. Long-term flexural strength of glassionomer cements. Biomaterials. 1991;12:658-660. Williams JA, Billington RW. Changes in compressive strength of glass-ionomer restorative materials with respect to time periods of 24 h to months. J Oral Rehabil. 1991;18:163-168. Bagheri R, Mese A, Burrow MF , et al. Comparison of the effect of storage media on shear punch strength of resin luting cements. J Dent. 2010;38:820-827. Fano L, Fano V, Ma W, et al. Hydrolytic degradation and cracks in resin-modified glassionomer cements. J Biomed Mater Res B Appl Biomater. 2004;69:87-93. Nakamura T, Wakabayashi K, Kinuta S, et al. Mechanical properties of new self-adhesive resin-based cement. J Prosthodont Res.
jdb.sums.ac.ir J Dent Biomater 2017;4(2)
2010;54:59-64. Hyun-Jin Kim, Rafat Bagheri, Young Kyung Kim, Jun Sik Son, Tae-Yub Kwon. Influence of Curing Mode on the Surface Energy and Sorption/Solubility of Dental Self-Adhesive Resin Cements. Materials (Basel). 2017 Feb; 10: 129. McCabe JF, Walls AW. Applied dental materials. 9th Edition. Blackwell: Oxford, UK; 2008. p. 274-285.. Oysaed H, Ruyter IE. Composites for use in posterior teeth: mechanical properties tested under dry and wet conditions. J Biomed Mater Res. 1986;20:261-271. Ferracane JL, Berge HX, Condon JR. In vitro aging of dental composites in water – effect of degree of conversion, filler volume, and filler/matrix coupling. J Biomed Mater Res. 1998;42:465-472. Wilson AD, McLean JW. Glass-ionomer cement. 1th edition. Chicago: Quintessence Publ Co.; 1988. p. 30-33 Phillips S, Bishop BM. An in vitro study of the effect of moisture on glass ionomer cement. Quintessence Int. 1985;16:175-177.